Straight Dagger Knife Blade Blank CPM154, 8.5"OAL, 4.25"Blade Length x 3/4"Blade Width, .110" thick
- Buy 3 for $21.16 each and save 5%
Straight Dagger Knife Blade
4.25"L x 3/4"W blade length and width
3qty - 3/16" Pin Holes
2qty - 7/64" Bolster Holes
Made in USA!
Note: this blade will need to be heat treated.
154CM, CPM154, ATS34 Heat Treating Information
All three of these, heat treat the same. After a full speed ramp up to temperature, they soak 45 minutes to an hour in the Evenheat Oven at 1950F degrees. Then they get placed still in the foil spine down then flat - on a 1 aluminum plate. The second aluminum plate is placed on top and pressure is applied. We used to use weights for the pressure, but now we use clamps. You are looking for good firm contact. If you are thinking hydraulics you are thinking WAY too much pressure. After 2 minutes (or less) they will be hand cool, and ready to remove from the foil for cryogenics. They dont have to go straight into cryo, but aim for something less than an hour from plate quenching. We use liquid nitrogen for cryo but dry ice in acetone will also do. The household freezer is no use at all. They probably only need a couple hours in cryo, but we leave them overnight.
The next morning, they will be in the range of RHC63+. After warming to room temperature, they get tempered. We temper twice at 500F degrees for two hours each time to get about RHC61. You can experiment for other hardness's but 61 is a very good target for these steels.
- Kirinite (TM) - Bengal Tiger - 1/8" Thick - Knife Handle Material
Starting at $13.87
- Rod - Stainless Steel 416 Rod - Pinstock
Starting at $0.99